(2) Polarization and EIS studies to evaluate the effect of aluminum concentration on the corrosion. . .. of Sn-3.7Ag-0.9Zn solder were decreased by the addition of 0.5 wt.% and 1 wt.% of Al. The effect of 0.1 wt.% and 0.2 wt.% Al on microstructure and mechanical properties of Sn-1.0Ag-0.5Cu was investigated by Dhafer et al. . They reported that the addition of Al resulted in larger and less-packed intermetallic compounds (IMCs), large primary β-Sn dendrites and shrunken interdendritic regions. Lee et al.  investigated the effect of Al addition on the wettability and drop impact reliability of SnAgCu solder. The addition of 0.005 wt.% to 0.02 wt.% Al into SAC105 resulted in decreased wetting time and increased wetting force. However, the amount of surface oxide was increased when Al content was over 0.1 wt.%, hence, resulted in poor wetting properties.. the corrosion resistance of solder materials using Gamry G300 Potentiostat/Galvanostat (Gamry Instruments, Inc., USA). The solders used in the corrosion tests were obtained commercially Sn-1.0Ag-0.5Cu, Sn-1.0Ag-0.5Cu-0.1Al, Sn-1.0Ag-0.5Cu-0.5Al and Sn-1.0Ag-0.5Cu1.0Al. A 3.5 wt.% NaCl solution was used as a corrosion medium to simulate sea water. After the solder materials were cut into blocks with specific dimensions (1 cm × 1 cm × 1 cm), a blind hole with a 1.6 mm diameter was drilled in the blocks surfaces for electrode connection. SiC paper grits 800, 1000, 1200 and 1500 were used to polish the sample surfaces. Those were washed with distilled water to remove impurities and then cleaned with acetone.. Mohanty et al.  have studied the effect of Al on the electrochemical corrosion behavior of a fiveelement alloy. They reported that an increase in Al content decreased the corrosion current density and corrosion rate of the five-element alloy (Sn-8.5Zn0.5Ag-XAl-0.5Ga). However, the corrosion potential value was shifted towards more noble value at higher Al content (1.5 wt.%). In another study, Mohanty et al.  reported that their results were opposite to the previous study. With an increase in Al content, the corrosion current density and corrosion rate of Sn-8.5Zn-XAl-0.5Ga was increased, while the corrosion potential shifted towards more negaFig. tive values. Many researchers [20, 22] have investigated the influence of Al on the microstructure and mechanical properties of the solder alloys. However, there is a lack of studies about the effect of these elements on the corrosion behavior of three-element alloys, especially SAC105. Therefore, in this study, the effect of Al concentration on the corrosion behavior of SAC105 solder alloy in 3.5 wt.% NaCl solution was investigated by polarization and electrochemical impedance spectroscopy (EIS) test.. 695. 1. Potentiodynamic polarization curves of SAC105, SAC105+0.1Al, SAC105+0.5Al and SAC105+1.0Al solder alloys in 3.5 wt.% NaCl solution.. Potentiodynamic polarization studies were carried out in a cell containing 3.5 wt.% NaCl solution. A platinum wire was used as a counter electrode, and a reference electrode used in our study was a saturated calomel electrode (SCE). The solder alloy placed inside the cell served as a working electrode with the area of 1 cm2 . Scanning of the potential was carried out from −1 to +1 V at a scan rate of 1 mV s−1 . The EIS measure2. Experimental ment was done at the corrosion potential in a frePotentiodynamic polarization test was con- quency range from 100 kHz down to 0.01 Hz. Afducted to obtain polarization curves in order to test ter the electrochemical corrosion test, the samples.
(3) 696. N. K. L IYANA et al.. The surface of the corroded samples covers by the insoluble hydroxide and creates a plateau region (DE) where the current density is found to be independent of potential. It should be noted that Al is the minor element in SAC105, so it is quickly depleted or blocked by Al(OH)3 on the surface. 3. Results and discussion Thus Sn, as the second most active material af3.1. Potentiodynamic polarization curves ter Al in this system, can be dissolved to Sn(II) The potential-current density profiles of the Sn- species [23, 24] according to the reactions disAg-Cu-XAl (X = 0, 0.1, 0.5, 1.0) solders obtained played below: by the potentiodynamic polarization studies car2OH− + Sn → Sn(OH)2 + 2e− (5) ried out in 3.5 wt.% NaCl solution are presented in Fig. 1. Since all corrosion tests were performed Sn(OH)2 → SnO + H2 O (6) in an aerated NaCl solution the cathodic branch of polarization curves may be ascribed to the disThe electrochemical data extracted from these solved oxygen reduction reaction: curves are summarized in Table 2. It is seen O2 + 2H2 O + 4e− → 4OH− (1) that the SAC105 solder alloy exhibits the corrosion potential of −668 mV (SCE). With the adThe potential at point B is referred to as Ecorr dition of 0.1 wt.% Al, the corrosion potential in(corrosion potential), where the extrapolated an- creases to −637 mV (SCE). However, as 0.5 wt.% odic and cathodic Tafel slopes intersect and the cur- and 1.0 wt.% Al is added to the SAC105 solrent becomes zero. Increasing the potential up to der alloy, the corrosion potential of the solder deEcorr may induce dissolution of Al. The anodic re- creases to −669 mV (SCE) and −692 mV (SCE), actions for dissolution of Al can occur by the fol- respectively. lowing steps : The corrosion-current density Icorr is determined at the intersection of the Tafel lines which Al(s) + OH− → Al(OH)ads + e− (2) represent the corrosion rate of the system. From Fig. 1, it is seen that the shapes of the polariza− − Al(OH)ads + OH → Al(OH)2ads + e (3) tion curves for SAC105 and SAC105 + 0.1Al solder alloys are almost similar and there is no significant difference of corrosion rate between these two (4) alloys. The corrosion current density of SAC105 Al(OH)2ads + OH− → Al(OH)3ads + e− solder alloy is 0.451 × 10−3 mA/cm2 , which is The active dissolution of Al can be explained slightly lower than that of 0.526 × 10−3 mA/cm 2 by the potential difference existing among the alloy for SAC105 + 0.1Al solder alloy. However, the adelements. Table 1 shows that the electrode potential dition of 0.5 wt.% and 1.0 wt.% Al into SAC105 values of Ag, Cu and Sn are much higher compared solder alloy shifts the corrosion current density to with that of Al. Thus, Al has been considered as the more positive values, which indicates an increase most active among these metals. As a result, Al acts in corrosion rate. The corrosion current densities as an anode in the alloy and, therefore, more easily of SAC105 + 0.5Al and SAC105+1.0Al solder aldissolves in corrosive conditions. loys are 11.1 × 10−3 and 11.6 × 10−3 mA/cm2 , reAl(OH)3 production and deposition causes Al spectively. Therefore, we can conclude that the addepletion. The active dissolution of Al contin- dition of Al tends to decrease the corrosion resisues with increasing potential until the hydroxide tance of the solder. These results are in accordance (OH− ) concentration reaches a critical value and with that obtained by Mohanty et al.  when they supersaturates the surface of the alloy at point C. investigated the effect of Al concentration on the surfaces were characterized by scanning electron microscopy (SEM) equipped with energy dispersive X-ray (EDX) analysis and X-ray Diffraction (XRD)..
(4) Polarization and EIS studies to evaluate the effect of aluminum concentration on the corrosion. . .. 697. Table 1. Electrode potential of solder elements. Reaction. Electrode potential [V]. Silver. Ag2+ + e− = Ag. + 0.7996. Copper. Cu+. e−. + = Cu Cu2+ + 2e− = Cu. +0.5210 +0.3419. Tin Aluminum. Sn2+ + 2e− = Sn Al3+ + 3e− =Al. −0.1375 −1.6600. Element. corrosion behavior of Sn-Zn-Al-Ga alloy. Mohanty et al.  reported that the corrosion current density and corrosion rate of Sn-8.5Zn-XAl-0.5Ga increased significantly with an increase in Al content. At potential more positive than B, corrosion rate increases and reaches a maximum at the passivation potential, C, which is presented by symbol, Epass and critical current density defined by symbol Icc . At the passivation potential, the transition from active dissolution occurs as the solid species (oxide/hydroxide of Al and Sn) become more stable than the parent metal ion . The surface of the electrode is covered by these oxide/hydroxides, thereby decreasing the current density with further increment in potential to point D (Fig. 1). The current density observed in the passive region DE in Fig. 1 is referred to as the passivation current density (Ipass ).. indicates the transpassive region which might be due to the breakdown of the passive film by incorporation of Cl− anion into the oxide layer, leading to localized corrosion. Previous study  reported that the film was mechanically broken due to the penetration of chloride ions into the oxide film and forming a solid metal chloride. The overall view from Fig. 1 shows that the addition of Al shifted the corrosion current density and passivation current density towards more positive values. This suggests that SAC105 + 1.0Al solder alloy has the lowest corrosion resistance. Higher content of Al in the Sn-1.0Ag-0.5Cu-XAl alloy enhances corrosion. These changes are also reflected in the corrosion rate as shown in Table 2.. 3.2.. Corrosion rate. The corrosion rate was obtained by Tafel fit using Gamry Echem Analyst DC105 software and the data are listed in Table 2. From Table 2, it is seen that SAC105 solder alloy shows the lowest corrosion rate, 0.07 mpy. When 0.1 wt.% of Al was added, the corrosion rate was slightly increased to 0.08 mpy. Corrosion rate of SAC105 solder alloy kept increasing to 1.44 mpy and 1.49 mpy when 0.5 wt.% and 1.0 wt.% Al were added, respectively. As a result, it can be concluded that SAC105 + 1.0Al solder alloy deteriorates and corrodes more rapidly with the low corrosion resistance and the highest corrosion rate.. From Table 2, it is seen that SAC105 solder exhibits the smallest critical current density (39.8 mA/cm2 ) and passivation current density (2.55 mA/cm2 ). The values of current density increase as Al is added into SAC105 solder. However, the current density is found to be the lowest for 0.1 wt.% Al in comparison to other alloys containing Al, thus indicating the stability of the passive film formed on the surface. Al content of 1.0 wt.% causes an increase in the passivation current density, thereby destabilizing the passive film which results in a higher rate of corrosion of the alloy. These results are in accordance with that ob- 3.3. Corrosion products tained by Mohanty et al. . They reported that solThe SEM micrograph in Fig. 2a shows the der with the lowest Al content has the lowest curformation of needle like corrosion products in rent density. SAC105 solder alloy. However, upon addition of Further increase in the potential beyond E aluminum, the size of the corrosion products seems causes a sharp increase in the current, which to be smaller (Fig. 2b and Fig. 2c)..
(5) 698. N. K. L IYANA et al.. Table 2. Potentiodynamic polarization parameters for SAC105, SAC105 + 0.1Al, SAC105 + 0.5Al and SAC105 + 1.0Al solder alloys in 3.5 wt.% NaCl solution. Materials SAC105 SAC105 + 0.1Al SAC105 + 0.5Al SAC105 + 1.0Al. Ecorr [mV]. Icorr [mA/cm2 ]. −668 0.451 × 10−3 −637 0.526 × 10−3 −669 11.100 × 10−3 −692 11.600 × 10−3. Icc [mA/cm2 ]. Ipass [mA/cm2 ]. Epass [mV]. ∆E [mV]. Corrosion rate [mpy]. 39.8 51.3 52.1 52.0. 2.55 2.98 24.30 38.80. −120.6 −110.8 −134.6 −158.5. 285.3 347.6 – –. 0.07 0.08 1.44 1.49. Samples which were potentiodynamically treated were subsequently subjected to X-ray diffraction (XRD) analysis as shown in Fig. 3. The XRD patterns reveal the presence of Sn3 O(OH)2 Cl2 (ICDD 00-039-0314), SnO (ICDD 98-006-019) and SnO2 (ICDD 98-000-9178) on the exposed surface of SAC105. Al(OH)3 (ICDD 98-000-6162) and Al2 O3 (ICDD 00-010-0173) were detected on the surfaces of Al-containing solder alloys. From the XRD analysis in Fig. 3, it is seen that Sn3 O(OH)2 Cl2 was undetectable when Al was added into SAC105 alloy. Instead, Al(OH)3 and Al2 O3 appear to be formed on the surfaces of SAC105 + 0.1Al, SAC105 + 0.5Al and SAC105 + 1.0Al solder alloys. These results are in accordance with the previous study conducted by Mohanty et al.  when they studied the effect of Al on the electrochemical corrosion behavior of Pb free Sn-8.5Zn-0.5Ag-XAl-0.5Ga solder in 3.5 wt.% NaCl solution. They reported that considerable aluminum segregation towards the surface occurred, predominantly as Al2 O3 /Al(OH)3 , with an increase in Al content to 1.5 wt.% in the fiveelement solder.. 3.4. Electrochemical troscopy (EIS). impedance. spec-. Fig. 4 displays the Nyquist plots for SAC105, SAC105 + 0.1Al, SAC105 + 0.5Al and SAC105 + 1.0Al solder alloys in 3.5 wt.% NaCl solution. As can be seen, the response of the system in the Nyquist complex plane is a semicircle arc for all materials whose diameter decreases with the addition of Al. The diameter of the Nyquist semicircle corresponds to the. corrosion resistance. It is important to remark that the highest semicircle arc corresponds to the best electrochemical corrosion behavior. In Fig. 4, it is seen that the loop diameter of SAC105 solder alloy is the highest. As Al was added into SAC105 alloy, the loop diameter decreased, which indicates the increased corrosion rate and thus, the reduction of corrosion resistance with the addition of Al. This observation permits to conclude that the SAC105 solder alloy has the best corrosion resistance as compared to others alloy. Fig. 5 shows the impedance spectra, presented as Bode plots, for SAC105, SAC105 + 0.1Al, SAC105 + 0.5Al and SAC105 + 1.0Al solder alloys in 3.5 wt.% NaCl solution. It is well-known that the corrosion resistance of solder alloys can be determined by log |Z| (Fig. 5a) and phase angle θmax (Fig. 5b) versus log frequency. Higher log |Z| and higher θmax represent better corrosion resistance. In the lower frequency region of the Bode plots (Fig. 5a), the log |Z| tends to decrease with the addition of Al and it has been tabulated in Table 3. It can be seen from Fig. 5 that the SAC105 solder alloy exhibits the highest magnitude of impedance, 4229 Ω·cm2 , and highest θmax , −77.28°, indicating the highest corrosion resistance which is attributed to the formation of comparatively more adherent and protective oxide film on the surface. Log |Z| and θmax tend to decrease with the addition of Al. This demonstrates that Al can reduce the corrosion resistance of the solder. From Table 3, it is seen that the values of log |Z| and θmax decrease to 3139 Ω·cm2 and −73.72°, respectively for SAC105 + 0.1Al and they keep to decrease to 1456 Ω·cm2 and −62.94°with the addition of 0.5 wt.% Al. At the highest concentration.
(6) Polarization and EIS studies to evaluate the effect of aluminum concentration on the corrosion. . .. 699. Fig. 3. X-ray diffraction scans after polarization for SAC105, SAC105 + 0.1Al, SAC105 + 0.5Al and SAC105 + 1.0Al solder alloys in 3.5 wt.% NaCl solution.. Fig. 4. Nyquist plot for SAC105, SAC105 + 0.1Al, SAC105 + 0.5Al and SAC105 + 1.0Al solder alloys in 3.5 wt.% NaCl solution.. of Al (1.0 wt.%), SAC105 alloy exhibits the lowest log |Z| (719.7 Ω·cm2 ) and θmax (−61.89°). It can be concluded that the addition of Al into the SAC105 solder causes a decrease in the corrosion resistance of the solder and SAC105 without Al addition exhibits the best corrosion resistance as compared to the other solders.. 4.. Conclusions. The following conclusions could be drawn from the present study Fig. 2. SEM micrographs (×4600) of SAC105 (a), SAC105 + 0.1Al (b) and SAC105 + 1.0Al (c) solder alloys after polarization test.. 1. The corrosion current densities of SAC105 + 0.1Al, SAC105 + 0.5Al and SAC105 + 1.0Al solder alloys.
(7) 700. N. K. L IYANA et al.. Table 3. Electrochemical impedance spectroscopy parameters for SAC105, SAC105 + 0.1Al, SAC105 + 0.5Al and SAC105 + 1.0Al solder alloys in 3.5 wt.% NaCl solution. Solder alloys SAC105 SAC105 + 0.1Al SAC105 + 0.5Al SAC105 + 1.0Al. Log |Z| [Ω·cm2 ]. θmax. [°]. 4229.0 3139.0 1456.0 719.7. −77.28 −73.72 −62.94 −61.89. aluminum and Sn matrix. Therefore, it can be concluded that the addition of Al decreases the corrosion resistance of the SAC105 solder alloy. 2. The common corrosion products form SAC105 include SnO, SnO2 and Sn3 O(OH)2 Cl2 . In our study, Sn3 O(OH)2 Cl2 was undetectable when Al was added into SAC105 alloy. Instead, Al(OH)3 and Al2 O3 appeared to be formed on SAC105 + 0.1Al, SAC105 + 0.5Al and SAC105 + 1.0Al solder surfaces. 3. Electrochemical impedance spectroscopy measurements showed that SAC105 solder alloy had the best electrochemical corrosion resistance. As Al was added into SAC105 alloy, the loop diameter was decreased which indicates the increased corrosion rate. Therefore, corrosion resistance was reduced with the addition of Al. This observation permits to conclude that the SAC105 solder alloy without Al addition has the best corrosion resistance as compared to others alloys. Fig. 5. 5 (a) magnitude Bode plot and (b) phase angle Bode plot for SAC105, SAC105 + 0.1Al, SAC105 + 0.5Al and SAC105 + 1.0Al solder alloys in 3.5 wt.% NaCl solution.. Acknowledgements The authors would like to acknowledge this project; the HIR project No: UM.C/625/1/HIR/MOHE/ENG/26. Author also would like to acknowledge the financial support provided by University of Malaya project (RP013B-13AET).. are 0.526 × 10−3 , 11.1 × 10−3 and References 11.6 × 10−3 mA/cm2 , respectively. With  M OHANTY U.S., L IN K.L., Appl. Surf. Sci., 252 (2006), 5907. the increase of aluminum concentration in  O SORIO W.R., S PINELLI J.E., A FONSO C.R.M., SAC105 solder alloy, the corrosion current P EIXOTO L.C., G ARCIA A., Electrochim. Acta, 56 density increases and polarization resistance (2011), 8891. decreases. This corrosion behavior seems  L EONARDO R.G., O SORIO W.R., P EIXOTO L.C., G ARCIA A., Mater. Charact., 61 (2010), 212. to be attributed to anodic dissolution of.
(8) Polarization and EIS studies to evaluate the effect of aluminum concentration on the corrosion. . ..  M OHANTY U.S., L IN K.L., J. Electrochem. Soc., 153 (2006), B319.  R AEDER C.H., F ELTON L.E., TANZI V.A., K NORR D.B., J. Electron. Mater., 23 (1994), 611.  T OMLINSON W.J., C OLLIER I., J. Mater.Sci., 22 (1987), 1835.  H ARADA M., S ATOH R., IEEE Trans. Compon., Hybrids, Manuf. Technol., 13 (1990), 736.  M C C ORMACK M., J IN S., J. Electron. Mater., 23 (1994), 635.  S ABRI M.F.M., D HAFER A.S., I RFAN A.B., S UHANA M.S., C HE F.X., TADASHI A., Mater. Charact., 78 (2013), 129.  X U L., PANG J.H.L., C HE F., J. Electron. Mater., 37 (2008), 880.  YOU T., K IM Y., K IM J., L EE J., J UNG B., M OON J., J. Electron. Mater., 38 (2009), 410.  L IU W., L EE N.C., JOM, 59 (2007), 26.  H UANG B., H WANG H.S., L EE N.C., Proc. Electronic Components and Technology Conf. (IEEE), 2007, 184.  B IRZER C., R AKOW B., S TEINER R., WALTER J., Proc. Electronics Packaging Technology Conf. (IEEE), 2005, 255.  Z HAO X.J., C AERS J.F.J.M., DE V RIES J.W.C., K LOOSTERMAN J., W ONG E.H., R AJOO R., Proc. Electronics Packaging Technology Conf. (IEEE), 2006, 174.. 701.  K IM D., S UH D., M ILLARD T., K IM H., K UMAR C., Z HU M., X U Y., Proc. Electronic Components and Technology Conf. (IEEE), 2007, 1614.  S UH D., K IM D. W., L IU P., K IM H., W ENINGER J.A., K UMAR C.M., P RASAD A., G RIMSLEY B.W., T EJADA H.B., Mater. Sci. Eng., A, (2007), 595.  K ITTIDACHA W., K ANJANAVIKAT A., VATTAANANIYOM K., Proc. Electronics Packaging Technology Conf. (IEEE), 2008, 1074.  K ARIYA Y., H OSSI T., T ERASHIMA S., TANAKA M., OTSUKA M., J. Electron. Mater., 33 (2004), 321.  W EI C., L IU Y.C., Y U L.M., C HEN H., WANG X., Microelectron. Reliab., 50 (2010), 1142.  D HAFER A.S., S ABRI M.F.M., I RFAN A.B., S UHANA M.S., C HE F.X., J. Mater. Sci. Mater. El., 23 (2012), 1988.  L EE Y.W., K IM I.H., K IM E.S., L EE J.H., M OON J.T., Proc. Electronics Packaging Technology Conf. (IEEE), 2010, 429.  S TIRRUP B.N., H AMPSON N.A., Surf. Technol., 5 (1977), 429.  D ROGOWSKA M., M ENARD H., B ROSSARD L., J. Appl. Electrochem., 21 (1991), 84.  P ISTORIUS P.C., B URSTEIN G.T., Corros. Sci., 38 (1994), 1525. Received 2016-04-15 Accepted 2017-11-08.